# CONSTITUTIVE ANALYSIS OF ELASTIC-PLASTIC ...esag. ... Constitutive analysis of elastic-plastic...

date post

19-Mar-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of CONSTITUTIVE ANALYSIS OF ELASTIC-PLASTIC ...esag. ... Constitutive analysis of elastic-plastic...

J. Mech. Phys. Solids, 1972, Vol. 20, pp. 401 to 413. Pergamon Press. Printed in Great Britain.

CONSTITUTIVE ANALYSIS OF ELASTIC-PLASTIC CRYSTALS AT ARBITRARY STRAIN

By R. HILL

Department of Applied Mathematics and Theoretical Physics, University of Cambridge

and

J. R. RICE

Division of Engineering, Brown University

(Received 16th August 1972)

SUMMARY

A GENERAL time-independent constitutive framework is constructed for crystals capable of crystallographic shearing. No restrictions are placed on their elasticity or on the amounts of slip. In deriving properly-objective relations due account is taken of the separate motions of the material and lattice. A precise specification of the structure of the flow rule leads to conditions for the existence of plastic potentials, as well as to an exact statement of the slip criterion required for normality of the plastic strain-increment in conjugate variables. Objective hardening laws are also examined and sufficiency conditions obtained for uniqueness of the slip magnitudes.

1. OBJECTIVES

WITHIN THE usual small-strain approximation there seems to be general agreement about a constitutive description of the mechanical properties of an elastic-plastic crystal at the macroscopic level. These are that (i) distortion of the lattice is effectively elastic; (ii) the crystal deforms also by simple shears relative to specific lattice planes and directions; (iii) such ‘slip systems’ are active only when the corresponding shear stresses attain critical values; and (iv) each value is a functional of the entire slip- history of the crystal.

It has been customary to treat the elasticity as linear and unaffected by slip, and to regard the lattice geometry as unaltered when stating the shears. The slip-induced rotation of the lattice relative to the material has often been ignored as well when computing increments of effective stress.

We put no restrictions here on the elasticity or the amounts of slip. Our intention is to construct a comprehensive constitutive framework in which the phenomena are analysed precisely.

2. POINT OF DEPARTURE

As a basis suitably general for our purpose we adopt the minimal framework outlined by HILL (1972).

This allows an arbitrary choice of strain measure e (HILL, 1968) relative to some ground state of the crystal. A conjugate measure of stress t in the deformed state is

28 401

402 R. HILL and J. R. RICE

defined by the requirement that de/p shall be the work per unit mass in any differential strain, where p is the ground-state density. Associated with such a (t, e) pair are fourth- rank tensors of moduli and compliances, LY and d say, which specify the in- stantaneous elastic behaviour under load.

It is supposed that crystallographic slip is the only mechanism responsible for inelastic behaviour. Then, under any incremental loading at constant temperature, we can always write

L?de - dt = C (My), de-&dt = c (pdy), (2.1) where

Iz=LY/l and

1

(2.2) p=&l,

with summation over the active slip systems. The dy’s are the incremental amounts of shear, reckoned with respect to the present lattice configuration, while the ii’s and k’s are second-rank symmetric tensors whose precise specification is our main objective.

For the moment we simply observe that C(pdy) is the residual increment of strain e after an infinitesimal loading and unloading cycle of the stress t, while ZZ(ldy) is the residual decrement of stress t after a like cycle of the strain e. These interpretations underline the relativity of the L’s and p’s to the chosen measures.

By contrast, however, it is known (HILL, 1968, 1972; and Appendix here) that the bilinear form

(Yde - dt)6e/p, (2.3)

where d and 6 are independent differentials, is invariant under change of measure. It follows that each Iz transforms in such a way as to preserve the Pfaffian kYe/p for arbitrary 6e; in short, each Iz transforms like t. Suppose, now, that LZ and A have the diagonal symmetry associated with the existence of a strain-energy function in some neighbourhood of the current stress. Then (2.3) is identical with

(de - .&“dt)&/p, (2.4)

where 6t = _Yde, and so each ~1 transforms so as to preserve pat/p for arbitrary 6t. Details of other consequences of changing the strain measure are recapitulated in

the Appendix. Here we need only mention the transformation formulae in the case when the ground state is not varied and, further, is taken coincident with the current state. For small additional strains any measure e can naturally be expanded as a power series in the logarithmic measure, e, say, beginning with the terms

e=e,+me,xe,+ . . . . (2.5)

where the cross signifies an inner product and m is some numerical coefficient (unity for the commonly adopted Green measure). In the ground state itself we have

de = de, and dt = dt,-m(axde+dexo),

dt, = 97, > (2.6)

where CT is the current Cauchy stress, t, is conjugate to e,, and 9~ is the Jaumann differential of Kirchhoff stress (HILL, 1968). This last formula is exact, and so independent of changes in measure that affect only terms beyond the second in the

Constitutive analysis of elastic-plastic crystals at arbitrary strain 403

series for e. It may be re-written as

dt = dt,-mYde, (2.7)

where 9’ is a fourth-rank symmetric tensor, which is evidently a linear function of o alone. By applying (2.7) with elastic increments, in particular, we obtain the trans- formation rule for instantaneous moduli:

8=_YO-mY. (2.8)

It follows that the transformation preserves symmetry of the type mentioned, when it exists. Also, for moderate values of m (of order unity in absolute magnitude), the differences in moduli are of the order of the applied stress and consequently proportionately small in metal crystals.

Lastly, by combining (2.7) and (2.8), we have

8de - dt = PO de, - dt, (2.9)

since terms in m cancel. Thus, when the current and ground states coincide, the Xs are actually invariant under change of measure. This conforms with the remark after (2.3), since every t = d when e = o. On the other hand, the p’s still alter, being given by &Iz where d is the inverse of 9 in (2.8).

3. CONSTRUCTION OF A FLOW RULE

(i) The elastoplastic behaviour of a crystal is governed by the geometry and orientation of its lattice. Since slip causes this to move through the material (as viewed macroscopically), we need to keep track of the separate deformations in the lattice and the material, and to distinguish stresses relative to either.

For the present we let both the strain measure and ground state be arbitrary. Then, if de is a differential strain of the material and d*e is the accompanying strain of the lattice,

de-d*e = C (vdy), (3.0

where the a’s are the associated measures of crystallographic unit shears (with respect to the deformed lattice).

Let dt and d*t denote increments in t reckoned relative to the material and lattice respectively. We make the distinction precise a little later. However, since any relative motion of the material and lattice is caused by slip alone, it is clear in advance that

dt - d*t = C (ady) (3.2)

with certain specifiable a’s, depending only on lattice geometry and the current stress and strain.

The preceding equations are primarily kinematic in character. We already have a constitutive connexion between dt and de, namely (2.1) which we repeat for convenience :

_!Zde - dt = C (Ady). (3.3)

It remains to state a constitutive connexion between d*t and d*e. This is necessarily of type

d*t - _Yd*e = C (/ldy) (3.4) with the same modulus tensor 9, since lattice and material deform as one in the absence of slip. The /?‘s represent a possible stiffening of the lattice due to microscopic

404 R. HILL and J. R. RICE

phenomena associated with continued slipping. That is, an extra increment of stress, X(/My) relatively to the lattice, would have to be applied to maintain its deformation as it was before the dy’s occurred.

We are now in a position to identify the I’s and $s in terms of the v’s, a’s and /?‘s, all of which may be regarded as known. Addition of (3.3) and (3.4) produces

_Y(de-d*e)-(dt-d*t) = C {(A+/?)dy).

Having regard to (3.1) and (3.2) it is apparent that we can set

Iz = (%+a)-p (3.5)

for each slip system. Further, the v’s and (as we shall see) also the a’s do not depend on the ratios of the dy’s, nor therefore in particular on how many systems are active simultaneously. Consequently neither do the Iz’s, unless it be via the B’s.

In passing, we recall that the residual strain after an infinitesimal cycle of stress t is Z((cldy) where, according to (3.2) and (3.5),

p = v-&(a+/?). (3.6)

Thus, what is commonly called ‘plastic’ deformation is not generally the resultant IZ(vdy) of the slips alone. In particular, no matter what stress measure is cycled, the residual strain-increment usually contains a dilatational component.

(ii) We return to the specification of the a’s in (3.2). For this purpose it is simplest to choose the ground state coincident with the current state. Then, by applying a standard formula, the Jaumann differentials of Kirchhoff stress with respect to the material and lattice are connected by

%--g*z = ax(d&d*Q-(de-d*O)xa (3.7)

Recommended

*View more*